PHYSICAL REVIEW B
VOLUME 60, NUMBER 10
1 SEPTEMBER 1999-II
Conduction channels and magnetoresistance in polycrystalline manganites
A. de Andrés, M. García-Hernández, and J. L. Martínez
Instituto de Ciencia de Materiales de Madrid (Consejo Superior de Investigaciones Científicas), Cantoblanco, E-28049 Madrid, Spain
Received 25 January 1999
We have performed magnetic and transport measurements on several series of La 0.7 Ca 0.3 MnO 3 polycrystalline
pellets and thin films. The aim is to discriminate the effects of structural and chemical disorder on the
electronic transport properties of polycrystalline manganites. We propose a macroscopic model that takes into
account that electric transport is dominated by the evolution with temperature and external magnetic field of
different kinds of parallel connected conduction channels. The relative weight of these channels is determining
the overall measured resistance, insulator-to-metal transition temperature, and magnetoresistance. We demonstrate
that transport properties of samples with the same magnetic behavior are dominated by the connectivity
between grains, but not to grain size effects, at least down to 12 nm grain diameter. The model reproduces very
well the magnetoresistance at low temperature for all measured samples with different grain sizes and grain
Manganese perovskites La 1x Ca x MnO 3 (ACa,Sr,
Ba...) have recently attracted much interest because of
their particular transport and magnetic properties. Their high
up to colossal magnetoresistance MR effect 1 make these
compounds promising regarding potential magnetic applications.
Ca-doped compounds with 0.15x0.5 present an
insulator-to-metal transition, at a temperature T IM , tightly
related to their para to ferromagnetic transition, at T c . Both
transitions occur at a temperature of about 265 K for the x
0.3 compound. The metallic ferromagnetic state is quite
well described by the double-exchange model, but polaronic
effects due to strong electron-phonon coupling and Jahn-
Teller distortions have also to be invoked in the insulator
regime, where the conduction is achieved by hopping of
small polarons. 2 These effects have also to be taken into
account even in compounds that are metallic in the paramagnetic
state, as those doped with Sr.
A great deal of interest arose in polycrystalline manganites
due to the high magnetoresistance that systems with
grain boundaries present at temperatures far from the magnetic
transition temperature: Single crystal and epitaxial film
magnetoresistance is maximum near T IM (T c ) and almost
zero at low temperatures; on the contrary, polycrystalline
samples present high magnetoresistance down to low
temperatures. 3,4 The effect of grain boundaries, tunnel junctions,
and grain size has been extensively studied. 5–7 Several
authors report on the decrease of the T IM for polycrystalline
systems 8–11 or films with microcracks 12 and related that to
grain-size effects, 4,11 or to the presence of insulating regions
at grain boundaries. 9 Magnetoresistance due to one single
boundary has been evidenced. 13,14 Kim et al. suggest that
intergranular resistance is probably the origin of the discrepancies
between infrared and dc resistivities. 15 Wang et al. 16
present the differences in the resistance with a 300 mT magnetic
field and without field between one sample obtained
by conventional sintering and another obtained by ‘‘partial
melting’’ and relate the differences to ‘‘weak or strong-link
grain boundaries.’’ Low-field magnetoresistance at low temperature
is now established to be a spin-polarized tunneling
process at grain boundaries 3,17–19 related to their half metallic
character. 20 The description of magnetoresistance in terms
of low and high field 11 or intrinsic and extrinsic
components 21 attempts to explain the observed behavior.
Nevertheless, several points remain open and some confusion
exists with respect to transport data in these systems.
While it is well established that the magnetic transition temperature
depends on the Mn 3 content, that can be altered by
different A-site doping or by changing the oxygen
stoichiometry, 22 the origin of the differences in the insulatorto-metal
transition temperature for samples with the same T c
is unclear. In fact, a model that reproduces the measured
resistivity and magnetoresistance as a function of the interfaces
and/or grain size, as well as an explanation for the large
increase of the magnetoresistance at low temperature for
fields above 1 T, when the magnetization is almost saturated,
as observed in all polycrystalline manganites, are still lacking.
In the present work we present a simple macroscopic
model with very few parameters based on the principles that
conduction is mainly achieved through the less resistive
channels, which correspond to clean contact areas between
grains. It is also assumed that all possible channels are parallel
connected. In the first part we demonstrate that electric
transport is dominated by the connectivity between the
grains. The model reproduces the dependence of the resistance
with and without magnetic field MR as a function of
the temperature as well as the shift or disappearance of the
insulator to metal transition. Afterwards we compare the
transport data of the pellets to those of polycrystalline thin
films. Finally, we show how the low temperature magnetoresistance
can be very well reproduced, on the same basis,
combining the measured variation of the magnetization with
the effect of an applied magnetic field on blocked Mn spins
at the grain surface. The external field leads to the opening of
new conduction channels parallel connected to those already
active at zero field. In summary, this model reproduces the
effect of structural and chemical disorder in transport data
when the magnetic behavior is the same. We will also dis-
0163-1829/99/6010/73287/$15.00 PRB 60 7328 ©1999 The American Physical Society
PRB 60 CONDUCTION CHANNELS AND MAGNETORESISTANCE . . .
cuss several cases reported in the literature that can be understood
taking into account the present model.
II. EXPERIMENTAL DETAILS
Three sets of samples were prepared in order to check the
effect of connectivity between grains, grain size, and chemical
disorder. Two series of pellets and one series of thin films
grown on Si100 were prepared.
It is well known that La compounds tend to degrade with
time when stored in air. We have hints of this degradation by
Raman spectroscopy and by the results we present here. The
surface of the grains tend to adsorb, probably, CO 2 and H 2 O
contained in the air. The process is reversible by heating at
about 1100 °C, above the temperature of dissociation of lanthanum
carbonate around 800 °C). It is expectable that the
smaller the grain size the greater the contamination, because
the surface to volume ratio increases as the size of the grains
Both series of ceramic samples are as follows: One half of
La 0.7 Ca 0.3 MnO 3 powder, with a mean grain size of several
microns, is annealed at 1200 °C for 24 h, in order to clean
the surface of the grains. The pellets obtained from this powder
are labeled C clean. The other half of the powder was
stored in air for several weeks samples labeled D: dirt surface.
With each kind of powder we made four pellets that
were sintered at different temperatures; 200, 500, 800, and
1100 °C for 4 h. The number used to label the sample indicates
its sintering temperature.
Powder x-ray-diffraction patterns were obtained for all
pellets showing identical lattice parameters, shapes, and
widths of the diffraction peaks. The size of the grains of the
starting powder is in the scale of the micron as observed with
an optical microscope. The effect of the sintering treatment
is not expected to increase the grain size: the grains of the
starting powder are quite large about 1.5 m) and the highest
sintering temperature was 1100 °C, well below the melting
point above 1600 °C). Therefore, the sintering effect
can only be to glue one grain to the other. In order to increase
the size of the grains, it would be necessary to rotate
the grains so as to align the crystallographic axes of two or
more grains. This process has certainly not taken place in our
samples due to the large starting grain size and ‘‘low’’ sintering
temperatures. SEM microphotographs of three of the
pellets C200, C800, and D1100 have been taken. The images
show that the mean grain size is identical for the three
samples, and can be estimated to be about 1.5 m. We can
ascertain that all the pellets have the same mean crystalline
grain size. The connectivity between grains will depend on
the sintering temperature while the quality of the grain surface
depends on the starting powder clean or dirty grains.
The effect of the grain size is checked by comparing these
ceramic samples to a series of polycrystalline thin films of
different grain sizes. The thin films were grown by dc sputtering
at room temperature on Si 100 substrates in a mixed
Ar and O 2 atmosphere ratio 4:1 and then annealed at
850 °C for 600 s. The films atomic-force microscopy images
show grains of rather spherical shape with mean diameters
between 12 and 80 nm depending on film thickness between
100 and 1200 nm. Grazing incidence and standard x-ray
diffraction of the thin films revealed their polycrystalline
FIG. 1. Derivative of the magnetization at 1000 Oe of several
representative pellets. Inset: hysteresis cycles of two pellets. The
samples are labeled with a letter D is the dirt surface, C is the clean
surface, and a number, which is the sintering temperature of the
character and expected lattice parameters for Ca concentration
of about 28%. The details of the growth, structure, morphology,
and transport properties have been presented
The magnetization measurements were performed either
in a superconducting quantum interference device magnetometer
for the thin films or in a physical properties measurement
system PPMS from Quantum Design pellets. The
transport measurements were all performed in the PPMS
with a standard four-probe configuration.
III. RESULTS AND DISCUSSION
First of all, magnetic and transport behavior of both series
of pellets, with the same grain size, are presented. Figure 1
shows the magnetic behavior of several representative pellets.
The magnetic transition temperature is identical for all
of them and, at 5 K, the magnetization is practically saturated
at about 1 T see inset. Figures 2a and 2b present
the resistance of the same samples, measured at 0 and 9 T,
normalized by their respective values at 300 K and 0 T. The
arrows indicate the maximum in the resistance corresponding,
in principle, to the insulator-to-metal transition. Notice
that the D200 sample does not even show a metallic regime.
The magnetic transition temperature (T c ) is also indicated. It
can easily be observed in Fig. 2 that, as the sintering temperature
decreases, the insulator-to-metal transition temperature
(T IM ) decreases and R(T)/R(300 K) dramatically increases
at low temperatures. Moreover, the resistance at 300
K increases several orders of magnitude not seen in Fig. 2
because data are normalized to R(300 K, 0 T). A similar
dependence of the resistance with temperature as that presented
by samples sintered between 200 and 800 °C have
been reported for thin films and powder samples with small
grain size, obtained by sol-gel techniques, and either have
7330 de ANDRÉS, GARCÍA-HERNÁNDEZ, and MARTÍNEZ
FIG. 3. Schema for the conduction in two granular systems with
a poor connectivity left and a better connectivity right. Lower
part: the equivalent circuits with two resistances in parallel: R M for
good channels and R I for bad channels. The curved arrows in the
upper part are related to good channels.
FIG. 2. Normalized resistance at 0 and 9Tfora two pellets,
both annealed at 1100 °C but with clean C1100 and dirt D1100
starting powders showing the effect of a dirt surface in the resistance
and b pellets annealed at different temperatures 200, 500,
800, and 1100 °C). c Magnetoresistance for three samples. Continuous
lines are the fits detailed in the text.
been related to grain-size effects or have been overlooked.
We will comment on this point later, but in the present series
of samples we do not have different oxygen content, except
in the contaminated D samples where the composition of the
surface layer of the grains is not known. Nevertheless, because
the magnetic transition temperature is identical for all
pellets, even for the dirt samples, the average oxygen content
is expected to be very nearly the nominal one.
We propose the following phenomenological model that
can explain the large differences in the measured electric
resistance, R(T), taking into account that magnetic properties
are identical for all pellets: Two kinds of conduction
channels are present in the samples and all of them are parallel.
One kind is related to the intrinsic transport properties
of the system and is achieved through good contacts between
grains. The other kind of channels show energy barriers that
inhibit metallic conduction at all temperatures due to poor
connectivity, disorder, and/or contamination. These defects
are mainly due to the fact that there are physical barriers
between grains because i the grains are not close enough,
ii their surface is contaminated, iii Mn environment at the
surface is not the same as that inside the grains; in all cases
Mn-O-Mn paths can be broken or distorted decreasing the
conductivity. The actual situation is probably very complicated
with a large distribution of barriers but, in fact, from
the conduction point of view, it is not so important: among
the different channels, the conduction will be effected
through the less resistive ones because these are parallel
channels. Moreover, as the temperature decreases, the available
thermal energy to overcome the barriers decreases exponentially
so the contribution to the conductivity of ‘‘bad
channels’’ decreases accordingly. On the other hand, depending
on the connectivity of the grains, which is determined
by the sintering temperature, and on the quality of the
surface, the effective section for ‘‘good’’ conduction, with
respect to that of other paths, changes from one sample to
another. Figure 3 illustrates this picture for electric transport.
For the present samples the effect of ‘‘contamination’’ is less
important than connectivity since R(T) curves are very similar
for pellets sintered at the same temperature, for example
D200 and C200, or D500 and C500. Only the best sintered
samples at 1100 °C) present a clear difference in their resistance
curves Fig. 2a: the metal-transition temperature
changes from 270 to 190 K for C1100 and D1100, respectively.
This means that conduction barriers due to bad
physical contacts between grains are higher than those related
to a contaminated surface. Obviously, if the surfaces of
the grains are more degraded than in the present samples, its
effect can be more important, as it can be the case for
samples with very small grain size obtained from ball milling
or sol-gel techniques. In any case both kinds of defects play,
qualitatively, the same role, and have to be very carefully
considered before trying to extract conclusions from resistance
data, especially when the magnetic transition temperature
of the samples are identical. Electric transport data can
be dominated by this kind of spurious effect.
This model can also be applied to Sr-doped manganites
which are nominally metallic above T c and where bad connectivity
and/or contamination of the grain surface can lead
to an apparent semiconductor behavior and to an increase of
the resistance, depending on the relation of the sections for
‘‘good’’ and ‘‘bad’’ channels. The explanation is valid also
for polycrystalline films with the same T c but different oxygen
content: the T c value is related to the composition of the
major part of the film, nevertheless small variation of the
oxygen content, localized at the grain surface will break the
Mn-O-Mn channels from one grain to the other increasing
the measured resistance.
Xiong et al. 24 have reported the resistivity curves for several
epitaxial Nd 0.7 Sr 0.3 MnO 3 films prepared changing the
oxygen pressure during the deposition. The data show that,
depending on the sample, the peak temperature at which the
PRB 60 CONDUCTION CHANNELS AND MAGNETORESISTANCE . . .
resistance is maximum varies from 170 down to 50 K, or
even lower. The authors propose that the films can be seen as
a paramagnetic matrix paralleled by ferromagnetic filamentary
paths, but they do not relate the transport changes to any
characteristic of the films. True epitaxial films with the correct
composition present a single-crystal behavior, so we
propose, in this case, that it is very probably related to a
variation in the oxygen content of the films. This can be
easily checked because T c would change from one film to
another depending on the oxygen content, disappointingly,
the authors do not give the magnetic transition temperatures
for the different films.
We show now that this model, with only two parameters,
can quantitatively very well reproduce the dependence of the
resistance with temperature, with and without external magnetic
field, of all pellets. In the present case, above T c , the
lowest barrier for conduction is that of polaron hopping from
one Mn to another, which is about 100 meV. 25 For the
present samples we have fit the paramagnetic phase data to a
semiconductor model obtaining an activation energy about
this value for all samples. The fit to a polaronic conduction
mechanism leads to a slightly different activation energy but
identical quality of the fit in the measured temperature range
up to 350 K. In fact, it is necessary to considerably enlarge
the temperature range towards high temperatures to be able
to discern between both conduction processes thermally activated
carriers or polaron hopping.
We model the measured resistance as two resistances in
parallel: 1/R(S m / m S i / i ) with resistivities m for
good channels which are metallic below T c ) and i bad
channels: always insulating, with an activation energy E i )
with effective sections S m and S i , respectively we consider
always the unit length. The resistivity of ‘‘good channels’’
( m ) should be that of a good quality single crystal, but we
do not have such a crystal, therefore, we take m (T)
(C1100,T)A exp(E a /k B T) i.e., the resistivity of our
best sample, in series with a component that takes into account
the low temperature below 50 K increase of the resistance.
This rise of the resistance is often observed and has
been related to the Coulomb blockade. This is probably the
process for very small grains but in the present case as for
many of the reported in the literature we associate this contribution
with small structural distortions at grain boundaries,
that give rise to small activation barriers E a and which are
observable only at low temperature where the ‘‘intrinsic’’
metallic resistivity is very low. This contribution to m (T) is
modulated by an amplitude factor A and we take E a 5 K
0.43 meV for all samples. The insulating paths are simply
modeled by a semiconductorlike resistivity: exp(E i /k B T)
with E i 100 meV the paramagnetic phase activation energy.
Continuous lines in Fig. 2b are the fits for several
samples at 0 and 9 T with this simple model, where the only
parameters are S m /S i and A. The activation energies (E i and
E a ) being the same for all samples. In order to fit the 9 T
measured resistance it is necessary to increase S m : as we
shall see later, the external magnetic field increases the effective
section for the good channels. The values for the
fitting parameters are collected in Table I. It can therefore be
concluded that i the observed phenomenology can be very
well understood with two kinds of parallel paths, ii it is
TABLE I. Parameters of the fits to resistance data presented in
Fig. 2. S m /S i is the ratio of the effective sections for ‘‘good’’ and
‘‘bad’’ conduction channels. A is the weight of the low-temperature
component to resistance.
Sample Magnetic field S m /S i A
C800 0 T 0.833 0
9T 1 0
D500 0 T 0.0435 0.1
9 T 0.111 0.1
D200 0 T 0.0125 1.8
9 T 0.0666 1.8
independent of the grain size or of the width of the claimed
grain shell. In turn, it depends on the fraction of the sample
with good conduction.
An early experiment, 26 that, in our opinion, supports this
model, presents the differences between dc and microwave
resistivities in polycrystalline Nd 0.7 Sr 0.3 MnO 3 . While dc resistivity
shows a slow decrease below T c and a relatively
high residual resistance at low temperature, the resistivity
obtained from microwave 10 GHz absorption shows a
single-crystal-like behavior: steep decrease below T c and
low resistivity at low temperature. The single-crystal-like behavior
can be understood taking into account that, at so high
frequencies, the major part of the carriers cannot cross the
boundaries from grain to grain, therefore the resistivity is
that of each grain which is, obviously, a small single crystal.
Very tightly related to these experiments are the comparison
of dc resistivity measurements to the conductivity extracted
from the far-infrared reflectivity at low temperatures, in the
metallic phase. 15 The dc resistivity is higher than that obtained
from the free-carrier density, because in the first case
the carriers have to cross the grain boundaries so the measured
resistance depends on the fraction of the sample with
good conduction. In fact, at low temperature, where the conduction
is effective basically only through good contacts, the
resistivity (R.S/l) obtained from the measured resistance
R and herein called the S m section, instead of that of the
whole sample, would be very similar to the values obtained
from microwave or infrared experiments. This point is to
stress that, in many cases, the resistivity obtained from the
resistance and the geometrical parameters of the sample and
the experiment is not describing an intrinsic property of the
samples, as it can be dominated by the quality of the sintering
process. Recently, an interesting experiment has been
reported 12 on artificially induced microcracks in epitaxial
films. The authors report a large increase of the ‘‘resistivity’’
and decrease of the insulator-to-metal transition temperature
for films with cracks compared to those without cracks, all of
them with the same magnetic transition temperature. This
behavior, again, can be explained with the present model: the
microcracks change the connectivity, i.e., the section for
Figure 2c presents the measured and calculated magnetoresistance
for D200 and C800 samples together with measured
MR for C1100 as a function of temperature. Note that
only by changing the relative weight of ‘‘good’’ and ‘‘bad’’
channels we can reproduce the enormous observed changes
in the shape of the magnetoresistance: As the connectivity
7332 de ANDRÉS, GARCÍA-HERNÁNDEZ, and MARTÍNEZ
FIG. 5. Magnetoresistance at 5Kofseveral pellets and a representative
thin film TF20. The labeling of the pellets is explained in
Fig. 1 caption.
FIG. 4. a Derivative of the magnetization at 1000 Oe and b
resistance at 0 and 9Tofathin film with 20 nm grains TF20.
decreases the magnetoresistance decreases near T c and increases
at low temperature. Therefore, grain boundaries are
the origin of the differences between the single crystal and
polycrystal behavior in two ways. This point is evidenced by
the variation of the resistance at low temperature when the
thermal activation of the carriers is very much limited with
the applied magnetic field. At low fields, up to the nearly
fully magnetization of the sample, the principal process in
electronic transport is the spin-polarized tunneling at grain
boundaries. Simultaneously, the progressive ordering of
some Mn blocked spins at the grain surface opens new channels
in parallel, which decrease more and more the resistance.
In order to demonstrate that the observed behavior in the
resistance is not due to grain-size effects, we present magnetic
and transport data for thin films with very small grain
size, down to 12 nm, all of them with the same T c and T IM .
Figure 4 shows data for a representative thin film (T c
242 K) with grains of about 20 nm. T IM and T c are nearly
identical indicating the good quality of the samples and a
good connectivity. In fact magnetoresistance at 5K or
equivalently R(H)/R(0) of C1100 and the thin film TF20
are identical Fig. 5. The slope of the high-field magnetoresistance
at 5 K reported for different manganites with grain
sizes above 500 nm are all nearly identical around 0.23 and
coincides with our data for the C1100 sample and for all our
thin films grain diameters between 80 and 12 nm.
In Fig. 5 we present the measured R(H)/R(0) at 5 K for
several pellets and a representative thin film in particular
with mean grain size of 20 nm. It is readily observed that
magnetoresistance of the TF20 thin film and C1100 pellet are
identical, while pellets with worse connectivity and/or contaminated
grain surface have a higher slope of R(H)/R(0) in
the high-field region.
It is important to stress that there can be grain-size effects
in the transport properties, as is the case, and, in principle,
these should be related to differences in the magnetic behavior.
For example, our thin films present a higher coercive
field than the pellets, and their magnetic transition is less
sharp, as observed comparing Figs. 1 and 2, these are, very
probably, grain-size effects. Moreover, the low-field MR,
which is related to a different behavior of the magnetization
M(H), is also dependent on the grain size. However, one
of our main points in this paper is to underline that other
effects, apart from grain size, can take place and, in fact, can
be dominating the electric transport.
Figure 6 shows C1100, D200, and TF20 measured magnetoresistance
together with a fit considering the following
mechanism: At low temperature the good channels give rise
to a magnetoresistance which is determined by the spinpolarized
tunneling between grains that depends on the angle
formed by the magnetic moments of these grains. 20 The
variation of this angle with the external magnetic field is
given by the measured magnetization M(H). Therefore, the
FIG. 6. Magnetoresistance of C1100 and D200 pellets and TF20
thin film gray symbols. Crosses are the magnetoresistance obtained
from the measured magnetization of a pellet inset of Fig. 1
and continuous lines black and white are the fits to the magnetoresistance
of three samples.
PRB 60 CONDUCTION CHANNELS AND MAGNETORESISTANCE . . .
conductivity for good channels G can be described by the
G H G 0CMH/M s 2 ,
where M s is the saturated magnetization and C is a constant
for a given temperature, and
R G H/R G 01/1CMH/M s 2 / G 0.
The related magnetoresistance, defined as MR(H)
100R G (H)/R G (0)1, is represented by crosses in Fig.
6. At the grain surface Mn spins can be blocked because, for
example, their environment is unbalanced or because of
magnetic anisotropy. In fact recent calculations demonstrate
that Mn ions of the outmost layer have their e g orbitals split,
their charge state modified, and a tendency to order
antiferromagnetically. 27 Magnetic measurements can be insensitive
to these disordered Mn spins, because the fraction
is very small, but the conduction at low temperature is drastically
reduced because one distorted Mn can close this conduction
channel. The hypothesis of this model is that the
magnetic field H aligns Mn spins blocked at the surface in
a linear way opening new conduction channels. The effective
section for electric conduction is S new (H) f •H, where f is a
constant. As these are parallel channels the inverse of the
resistances are added and we obtain
RH/R01/1„C/ G 0…„MH/M s … 2 1 f •H/S G ,
where S G , the good section for conduction at H0, depends
on the connectivity and contamination of the sample. In the
fits in Fig. 6: C/S G (0)0.33 for the three samples and
f /S G 0.068 for the C1100 and TF20 samples and 0.14
for the D200 sample, which is consistent with the idea that
the effective section for good conduction (S G ) of sample
C1100 is larger than that for D200. Note that high-field magnetoresistance
is not linear and that this model fits perfectly
the data in the whole measured magnetic field range for all
samples with only one parameter ( f /S G ).
In the present paper we have shown that the interpretation
of transport data has to be very carefully done. A T IM considerably
lower than T c together with a high resistivity at
low temperature is an indication of bad connectivity between
grains and not a grain-size effect. It has to be taken into
account that the conduction is achieved by parallel channels
and that the resistivity of these channels vary in a different
way with temperature depending on whether the metallic regime
is reached or not. The section for metallic conduction is
determined by the connectivity between grains that depends
on how good is the sintering and/or the contamination of the
grain surface. The effect of an external magnetic field is to
align blocked spins at the surface of the grains in a linear
way opening new conduction channels. Mn ions at the surface
can block the conduction if their e g levels are split introducing
an activation barrier therefore increasing drastically
the resistance as temperature decreases. This model is
valid for all granular systems whose main transport mechanism
is spin-polarized tunneling.
We thank L. Brey and F. Guinea for fruitful discussions,
L. Vazquez for AFM measurements, and J.M. Alonso for
preparing manganite powder. This work was supported by
CICyT under Contract Nos. MAT96-0395 and MAT97-725.
1 S. Jin, T. H. Tiefel, M. MacCormack, R. A. Fastnacht, R.
Ramesh, and L. H. Chen, Science 264, 413 1994.
2 M. R. Ibarra and J. M. de Teresa, in Giant Magnetoresistance and
Related Properties of Metal Oxides, edited by C. N. R. Rao and
B. Raveau World Scientific, Singapore, in press.
3 H. Y. Hwang, S. W. Cheong, N. P. Ong, and B. Batlogg, Phys.
Rev. Lett. 77, 2041 1996.
4 A. Gupta, G. Q. Gong, G. Xiao, P. R. Duncombe, P. Lecoeur, P.
Trouilloud, Y. Y. Wang, V. P. Dravid, and J. Z. Sun, Phys. Rev.
B 54, 156291996.
5 Y. Lu, X. W. Li, G. Q. Gong, G. Xiao, A. Gupta, P. Lecoeur, J.
Z. P. Sun, Y. Y. Wang, and V. P. Dravid, Phys. Rev. B 54, 8357
6 M. Viret, M. Drouet, J. Nassar, J. P. Contour, C. Fermon, and A.
Fert, Europhys. Lett. 5, 545 1997.
7 P. Lyu, D. Y. Xing, and J. M. Dong, Phys. Rev. B 58, 541998.
8 R. Ramesh, R. Mahendiran, A. K. Raychaudhuri, and C. N. R.
Rao, Appl. Phys. Lett. 68, 2291 1996.
9 S. Pignard, H. Vincent, J. P. Senateur, K. Frohlich, and J. Souc,
Appl. Phys. Lett. 73, 999 1998.
10 R. D. Sánchez, J. Rivas, C. Vázquez-Vázquez, A. López-
Quintela, M. T. Causa, M. Tovar, and S. Oseroff, Appl. Phys.
Lett. 68, 134 1996.
11 Ll. Balcells, J. Fontcuberta, B. Martínez, and X. Obradors, Phys.
Rev. B 58, 146971998.
12 K. M. Satyalakshmi, B. Fisher, L. Patlagan, G. Koren, E. Sheriff,
R. Prozorov, and Y. Yeshurun, Appl. Phys. Lett. 73, 402 1998.
13 K. Steenbeck, T. Eick, K. Kirsch, K. Odonnell, and E. Steinbeiss,
Appl. Phys. Lett. 71, 968 1997.
14 N. D. Mathur, G. Burnell, S. P. Isaac, T. J. Jackson, B. S. Teo, J.
L. Mac Manusdriscoll, L. F. Cohen, J. E. Evetts, and M. G.
Blamire, Nature London 387, 266 1997.
15 K. H. Kim, J. Y. Gu, H. S. Choi, D. J. Eom, J. H. Jung, and T. W.
Noh, Phys. Rev. B 55, 4023 1997.
16 X. L. Wang, S. X. Dou, H. K. Liu, M. Ionescu, and B. Zeimetz,
Appl. Phys. Lett. 73, 396 1998.
17 X. W. Li, A. Gupta, G. Xiao, and G. Q. Gong, Appl. Phys. Lett.
71, 1124 1997.
18 R. Shreekala, M. Rajeswari, K. Ghosh, A. Goyal, J. Y. Gu, C.
Kwon, Z. Trajanovic, T. Boettcher, R. L. Greene, R. Ramesh,
and T. Venkatesan, Appl. Phys. Lett. 71, 282 1997.
19 J. M. D. Coey, Philos. Trans. R. Soc. London, Ser. A 356, 1539
20 J. H. Park, E. Vescovo, H. J. Kim, C. Kwon, R. Ramesh, and I.
Veukatesan, Nature London 392, 794 1998.
21 P. Raychaudhuri, K. Sheshadri, P. Taneja, S. Bandyopaghyay, P.
Ayyub, A. K. Nigam, and R. Pinto, Phys. Rev. B 59, 13919
22 H. L. Ju, J. Gopalakrishnan, J. L. Peng, Qi Li, G. C. Xiong, T.
7334 de ANDRÉS, GARCÍA-HERNÁNDEZ, and MARTÍNEZ
Venkatesan, and R. L. Greene, Phys. Rev. B 51, 6143 1995.
23 M. García-Hernández, J. L. Martínez, A. de Andrés, L. Vázquez,
E. Herrero, and J. M. Alonso, J. Magn. Magn. Mater. 196-197,
24 G. C. Xiong, S. M. Bhagat, Q. Li, M. Domínguez, H. L. Ju, R. L.
Greene, T. Venkatesan, J. M. Byers, and M. Rubinstein, Solid
State Commun. 97, 599 1996.
25 I. O. Troyanchuk, Zh. Éksp. Teor. Fiz. 102, 251 1992 Sov.
Phys. JETP 75, 132 1992.
26 M. Domínguez, S. M. Bhagat, S. E. Lofland, J. S. Ramachandran,
G. C. Xiong, H. L. Ju, T. Venkatesan, and R. L. Greene, Europhys.
Lett. 32, 349 1995.
27 M. J. Calderón, L. Brey, and F. Guinea, Phys. Rev. B 60, 6698